Purification of deteriorated liquid crystals by employing ... Purification of deteriorated liquid...
Embed Size (px)
Transcript of Purification of deteriorated liquid crystals by employing ... Purification of deteriorated liquid...
Purification of deteriorated liquid crystals by employing porous metal–organic- framework/polymer composites
Tsung-Yu Tasi,1 Po-Chang Wu,2 Kun-Ting Liao,1 Hsi-Ya Huang,3,4 Chia-Her Lin,3,4 Jy-Shan Hsu,1,4,5,6 and Wei Lee2,5,*
1Department of Physics, Chung Yuan Christian University, Chungli 32023, Taiwan 2Institute of Imaging and Biomedical Photonics, College of Photonics, National Chiao Tung University, Guiren Dist.,
Tainan 71150, Taiwan 3Department of Chemistry, Chung Yuan Christian University, Chungli 32023, Taiwan
4Center for Nanotechnology, Chung Yuan Christian University, Chungli 32023, Taiwan 5These authors contributed equally firstname.lastname@example.org (J.-S. Hsu)
*email@example.com (W. Lee)
Abstract: This study demonstrates the effectual purification of degraded nematic liquid crystals (LCs) by introducing metal–organic framework (MOF) into the copolymer with either negatively charged 2-acrylamido-2- methylpropane sulfonic acid (AMPS) or positively charged (vinylbenzyl) trimethylammonium chloride (VBTA). Experimental results show that the ion elimination is primarily achieved by the nanoporous MOF itself while AMPS or VBTA plays an important role in functionalizing MOF with hydrophilicity. It was found that the overall ion-removal efficacy of either MOF/polymer-AMPS or MOF/polymer-VBTA composite is higher than that of the pristine MOF counterpart. ©2014 Optical Society of America OCIS codes: (160.3710) Liquid crystals; (160.4890) Organic materials; (160.5470) Polymers; (230.3720) Liquid-crystal devices.
References and links 1. C.-N. Lei, L.-M. Whang, and P.-C. Chen, “Biological treatment of thin-film transistor liquid crystal display
(TFT-LCD) wastewater using aerobic and anoxic/oxic sequencing batch reactors,” Chemosphere 81(1), 57–64 (2010).
2. W. Lee, C.-T. Wang, and C.-H. Lin, “Recovery of the electrically resistive properties of a degraded liquid crystal,” Displays 31(3), 160–163 (2010).
3. C.-T. Huang, K.-T. Liao, C.-H. Lin, J.-S. Hsu, and W. Lee, “Improved electric properties of degraded liquid crystal using metal–organic frameworks,” Appl. Phys. Express 6(12), 121701 (2013).
4. H.-Y. Hung, C.-W. Lu, C.-Y. Lee, C.-S. Hsu, and Y.-Z. Hsieh, “Analysis of metal ion impurities in liquid crystals using high resolution inductively coupled plasma mass spectrometry,” Anal. Methods 4(11), 3631–3637 (2012).
5. S. H. Perlmutter, D. Doroski, and G. Moddel, “Degradation of liquid crystal device performance due to selective adsorption of ions,” Appl. Phys. Lett. 69(9), 1182–1184 (1996).
6. V. A. Tsvetkov and O. V. Tsvetkov, “Ions influence on electrooptical characteristics of NLC,” Mol. Cryst. Liq. Cryst. (Phila. Pa.) 368(1), 625–632 (2001).
7. L. O. Palomares, J. A. Reyes, and G. Barbero, “Optical response of a nematic sample submitted to a periodic external electric field: role of the ionic impurities,” Phys. Lett. A 333(1-2), 157–163 (2004).
8. C. Colpaert, B. Maximus, and A. De Meyere, “Adequate measuring techniques for ions in liquid crystal layers,” Liq. Cryst. 21(1), 133–142 (1996).
9. H.-H. Liu and W. Lee, “Time-varying ionic properties of a liquid-crystal cell,” Appl. Phys. Lett. 97(2), 023510 (2010).
10. B.-R. Jian, C.-Y. Tang, and W. Lee, “Temperature-dependent electrical properties of dilute suspensions of carbon nanotubes in nematic liquid crystals,” Carbon 49(3), 910–914 (2011).
11. P.-C. Wu and W. Lee, “Phase and dielectric behaviors of a polymorphic liquid crystal doped with graphene nanoplatelets,” Appl. Phys. Lett. 102(16), 162904 (2013).
12. P.-S. Chen, C.-C. Huang, Y.-W. Liu, and C.-Y. Chao, “Effect of insulating-nanoparticles addition on ion current and voltage-holding ratio in nematic liquid crystal cells,” Appl. Phys. Lett. 90, 21111 (2007).
#229226 - $15.00 USD Received 8 Dec 2014; revised 23 Feb 2015; accepted 23 Feb 2015; published 25 Feb 2015 (C) 2015 OSA 1 Mar 2015 | Vol. 5, No. 3 | DOI:10.1364/OME.5.000639 | OPTICAL MATERIALS EXPRESS 639
13. C.-Y. Tang, S.-M. Huang, and W. Lee, “Analysis of defect mode switching response time in one-dimensional photonic crystal with a nematic liquid crystal defect layer,” J. Phys. D Appl. Phys. 44, 355102 (2011).
14. H.-Y. Jung, H.-J. Kim, S. Yang, Y.-G. Kang, B.-Y. Oh, H.-G. Park, and D.-S. Seo, “Enhanced electro-optical properties of Y2O3 (yttrium trioxide) nanoparticle-doped twisted nematic liquid crystal devices,” Liq. Cryst. 39(7), 789–793 (2012).
15. H.-K. Chung, H.-G. Park, Y.-S. Ha, J.-M. Han, J.-W. Lee, and D.-S. Seo, “Superior electro-optic properties of liquid crystal system using cobalt oxide nanoparticle dispersion,” Liq. Cryst. 5(5), 632–638 (2013).
16. H.-Y. Huang, C.-L. Lin, C.-Y. Wu, Y.-J. Cheng, and C.-H. Lin, “Metal organic framework-organic polymer monolith stationary phases for capillary electrochromatography and nano-liquid chromatography,” Anal. Chim. Acta 779, 96–103 (2013).
17. G. Férey, C. Mellot-Draznieks, C. Serre, F. Millange, J. Dutour, S. Surblé, and I. Margiolaki, “A chromium terephthalate-based solid with unusually large pore volumes and surface area,” Science 309(5743), 2040–2042 (2005).
18. D.-Y. Hong, Y.-K. Hwang, C. Serre, G. Ferey, and J.-S. Chang, “Porous chromium terephthalate MIL-101 with coordinatively unsaturated sites: surface functionalization, encapsulation, sorption and catalysis,” Adv. Funct. Mater. 19(10), 1537–1552 (2009).
19. G. Barbero and A. L. Alexe-Ionescu, “Role of the diffuse layer of the ionic charge on the impedance spectroscopy of a cell of liquid,” Liq. Cryst. 32(7), 943–949 (2005).
20. F.-C. Lin, P.-C. Wu, B.-R. Jian, and W. Lee, “Dopant effect and cell-configuration-dependent dielectric properties of nematic liquid crystals,” Adv. Cond. Mat. Phys. 2013, 271574 (2013).
21. W. Lee, C.-T. Huang, K.-T. Liao, J.-S. Hsu, and C.-H. Lin, “Metal–organic frameworks for regeneration of degraded liquid crystal,” Mol. Cryst. Liq. Cryst. (Phila. Pa.) 601(1), 88–96 (2014).
22. J. Yang, Q. Zhao, J. Li, and J. Dong, “Synthesis of metal–organic framework MIL-101 in TMAOH-Cr(NO3)3- H2BDC-H2O and its hydrogen-storage behavior,” Microporous Mesoporous Mater. 130(1-3), 174–179 (2010).
23. M. Suresh, B. David Raju, K. S. Rama Rao, K. R. Reddy, M. L. Kantam, and P. Srinivasu, “Metal organic framework MIL-101(Cr) for dehydration reactions,” J. Chem. Sci. 126(2), 527–532 (2014).
Liquid crystal displays (LCDs) are currently the most dominant type of flat-panel displays on the markets. Applications of human–machine interfaces increase numerously in a variety of commercially electronic and information-content products, such as digital cameras, mobile phones, notebooks, tablets, personal computers, and high-definition televisions. With growing popularity of LCD-related products, the increasing amount of waste materials, especially those received as leftovers from the production line, has emerged as one of critical issues in LC and related industries due to cost consideration and environmental protection . In view of the fabrication process of LCDs, a certain amount of LC remnants or spills is inevitable in the stage of panel-filling procedure regardless of the injection approach used. Such LC leftovers, in contact with the surrounding environment, are often contaminated as evidenced by the increasing content of ion impurities, most likely originating from the dissemination of atmospheric moistures and dust particles from air into LCs. It has been elucidated that the pollutants in degraded LCs are primarily composed of hydrogen cations and hydroxyl anions dissociated from water molecules as well as of metal cations [2-4]. Consequently, severe migration of mobile ions under an applied voltage could generate a considerable ionic effect in a LCD, causing image sticking and, in turn, detrimental display performance [5-8]. Although the adoption of LC materials with high resistivity as well as low ion density is the most reliable strategy to reduce the unwanted ionic effect in LCDs, the LC leftovers from the production line are not reusable in consideration of their loss of material integrity. Thus far, several potential non-synthesis approaches involving trapping or restraining the transport of ions have been extensively reported through the dispersion of specific nanomaterials in ion- rich LCs [9-15]. Disadvantageously, nanodopants suspended in LCs over time have a strong tendency to aggregate, implying that their long-term stability would be challengeable.
With the purpose toward the purification and recycle of LC leftovers obtained from flat- panel production lines, we have demonstrated in our previous work that soaking porous metal–organic frameworks (MOFs) as desiccants in LCs is a simple, feasible and cost- effective approach for the recovery of electrical or electrically resistive properties of degraded LCs . Owing to the unusual nanoporous structures and excellent water-sorption ability, it has been confirmed that MOFs can serve as useful purifiers for effective absorption of ion
#229226 - $15.00 USD Received 8 Dec 2014; revised 23 Feb 2015; accepted 23 Feb 2015; published 25 Feb 2015 (C) 2015 OSA 1 Mar 2015 | Vol. 5, No. 3 | DOI:10.1364/OME.5.000639 | OPTICAL MATERIALS EXPRESS 640
impurities in LCs. Nevertheless, when a MOF material in the powder form is immersed in LC for a period of time, an additional fine filtrating procedure must be performed to extract the purified LC from the LC–MOF “mixture”. To further enh